#------------------------------------------------------------------------------
#$Date: 2016-03-23 21:04:08 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179438 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/35/4333599.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4333599
loop_
_publ_author_name
'M. Falmbigl'
'F. Kneidinger'
'M. Chen'
'A. Grytsiv'
'H. Michor'
'E. Royanian'
'E. Bauer'
'H. Effenberger'
'R. Podloucky'
'P. Rogl'
_publ_section_title
;
 Cage-Forming Compounds in the Ba-Rh-Ge System: From Thermoelectrics to
 Superconductivity
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              931
_journal_page_last               943
_journal_paper_doi               10.1021/ic302139r
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'Ba8 Ge45 Rh'
_chemical_formula_weight         4468.18
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           223
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   10.693(2)
_cell_length_b                   10.693(2)
_cell_length_c                   10.693(2)
_cell_measurement_temperature    473(2)
_cell_volume                     1222.6(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      473(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0441
_diffrn_reflns_av_sigmaI/netI    0.0322
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            1646
_diffrn_reflns_theta_full        34.94
_diffrn_reflns_theta_max         34.94
_diffrn_reflns_theta_min         2.69
_exptl_absorpt_coefficient_mu    33.807
_exptl_absorpt_correction_T_max  0.4303
_exptl_absorpt_correction_T_min  0.2827
_exptl_crystal_density_diffrn    6.069
_exptl_crystal_F_000             1933
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.390
_refine_diff_density_min         -1.091
_refine_diff_density_rms         0.218
_refine_ls_extinction_coef       0.00010(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.162
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     18
_refine_ls_number_reflns         514
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.162
_refine_ls_R_factor_all          0.0638
_refine_ls_R_factor_gt           0.0319
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+11.2794P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0456
_refine_ls_wR_factor_ref         0.0502
_reflns_number_gt                351
_reflns_number_total             514
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302139r_si_002_2.cif
_cod_data_source_block           k1_200K
_cod_original_cell_volume        1222.5(4)
_cod_database_code               4333599
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'x+1/2, z+1/2, -y+1/2'
'-x+1/2, z+1/2, y+1/2'
'-x+1/2, -z+1/2, -y+1/2'
'x+1/2, -z+1/2, y+1/2'
'z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, x+1/2'
'-z+1/2, -y+1/2, -x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y-1/2, -x-1/2, z-1/2'
'y-1/2, x-1/2, z-1/2'
'-y-1/2, x-1/2, -z-1/2'
'y-1/2, -x-1/2, -z-1/2'
'-x-1/2, -z-1/2, y-1/2'
'x-1/2, -z-1/2, -y-1/2'
'x-1/2, z-1/2, y-1/2'
'-x-1/2, z-1/2, -y-1/2'
'-z-1/2, -y-1/2, x-1/2'
'-z-1/2, y-1/2, -x-1/2'
'z-1/2, -y-1/2, -x-1/2'
'z-1/2, y-1/2, x-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 0.0000 0.0000 0.0000 0.0119(2) Uani 1 24 d S
Ba2 Ba 0.2500 0.0000 0.5000 0.0357(3) Uani 1 8 d S
Rh1 Rh 0.2500 0.5000 0.0000 0.0112(6) Uani 0.20 8 d SP
Ge2 Ge 0.2500 0.5000 0.0000 0.0112(6) Uani 0.450(6) 8 d SP
Ge1 Ge 0.18361(4) 0.18361(4) 0.18361(4) 0.01436(17) Uani 1 3 d S
Ge3 Ge 0.0000 0.1150(3) 0.3079(5) 0.0131(6) Uiso 0.59(2) 2 d SP
Ge4 Ge 0.0000 0.1321(6) 0.3330(8) 0.0177(8) Uiso 0.41(2) 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rh Rh -1.1178 0.9187 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Ge1 Ba1 Ge1 180.00(2) . 25
Ge1 Ba1 Ge1 70.5 . 28
Ge1 Ba1 Ge1 109.5 25 28
Ge1 Ba1 Ge1 109.5 . 4
Ge1 Ba1 Ge1 70.5 25 4
Ge1 Ba1 Ge1 180.00(2) 28 4
Ge1 Ba1 Ge1 70.5 . 27
Ge1 Ba1 Ge1 109.5 25 27
Ge1 Ba1 Ge1 109.5 28 27
Ge1 Ba1 Ge1 70.5 4 27
Ge1 Ba1 Ge1 109.5 . 3
Ge1 Ba1 Ge1 70.5 25 3
Ge1 Ba1 Ge1 70.5 28 3
Ge1 Ba1 Ge1 109.5 4 3
Ge1 Ba1 Ge1 180.00(4) 27 3
Ge1 Ba1 Ge1 70.5 . 26
Ge1 Ba1 Ge1 109.5 25 26
Ge1 Ba1 Ge1 109.5 28 26
Ge1 Ba1 Ge1 70.5 4 26
Ge1 Ba1 Ge1 109.5 27 26
Ge1 Ba1 Ge1 70.5 3 26
Ge1 Ba1 Ge1 109.5 . 2
Ge1 Ba1 Ge1 70.5 25 2
Ge1 Ba1 Ge1 70.5 28 2
Ge1 Ba1 Ge1 109.5 4 2
Ge1 Ba1 Ge1 70.5 27 2
Ge1 Ba1 Ge1 109.5 3 2
Ge1 Ba1 Ge1 180.00(4) 26 2
Ge1 Ba1 Ge3 42.026(17) . .
Ge1 Ba1 Ge3 137.974(17) 25 .
Ge1 Ba1 Ge3 42.026(17) 28 .
Ge1 Ba1 Ge3 137.974(17) 4 .
Ge1 Ba1 Ge3 70.19(3) 27 .
Ge1 Ba1 Ge3 109.81(3) 3 .
Ge1 Ba1 Ge3 109.81(3) 26 .
Ge1 Ba1 Ge3 70.19(3) 2 .
Ge1 Ba1 Ge3 137.974(17) . 33
Ge1 Ba1 Ge3 42.026(17) 25 33
Ge1 Ba1 Ge3 109.81(3) 28 33
Ge1 Ba1 Ge3 70.19(3) 4 33
Ge1 Ba1 Ge3 70.19(3) 27 33
Ge1 Ba1 Ge3 109.81(3) 3 33
Ge1 Ba1 Ge3 137.974(17) 26 33
Ge1 Ba1 Ge3 42.026(17) 2 33
Ge3 Ba1 Ge3 109.13(3) . 33
Ge1 Ba1 Ge3 137.974(17) . 29
Ge1 Ba1 Ge3 42.026(17) 25 29
Ge1 Ba1 Ge3 70.19(3) 28 29
Ge1 Ba1 Ge3 109.81(3) 4 29
Ge1 Ba1 Ge3 137.974(17) 27 29
Ge1 Ba1 Ge3 42.026(17) 3 29
Ge1 Ba1 Ge3 109.81(3) 26 29
Ge1 Ba1 Ge3 70.19(3) 2 29
Ge3 Ba1 Ge3 109.13(3) . 29
Ge3 Ba1 Ge3 70.87(3) 33 29
Ge1 Ba1 Ge3 137.974(17) . 25
Ge1 Ba1 Ge3 42.026(17) 25 25
Ge1 Ba1 Ge3 137.974(17) 28 25
Ge1 Ba1 Ge3 42.026(17) 4 25
Ge1 Ba1 Ge3 109.81(3) 27 25
Ge1 Ba1 Ge3 70.19(3) 3 25
Ge1 Ba1 Ge3 70.19(3) 26 25
Ge1 Ba1 Ge3 109.81(3) 2 25
Ge3 Ba1 Ge3 180.0 . 25
Ge3 Ba1 Ge3 70.87(3) 33 25
Ge3 Ba1 Ge3 70.87(3) 29 25
Ge4 Ba2 Ge4 171.4(3) 41_666 2
Ge4 Ba2 Ge4 125.41(6) 41_666 .
Ge4 Ba2 Ge4 47.5(2) 2 .
Ge4 Ba2 Ge4 47.5(2) 41_666 42_666
Ge4 Ba2 Ge4 125.41(6) 2 42_666
Ge4 Ba2 Ge4 99.80(6) . 42_666
Ge4 Ba2 Ge4 61.1(3) 41_666 18_545
Ge4 Ba2 Ge4 125.41(6) 2 18_545
Ge4 Ba2 Ge4 171.4(3) . 18_545
Ge4 Ba2 Ge4 80.85(9) 42_666 18_545
Ge4 Ba2 Ge4 99.80(6) 41_666 26_556
Ge4 Ba2 Ge4 80.85(9) 2 26_556
Ge4 Ba2 Ge4 61.1(3) . 26_556
Ge4 Ba2 Ge4 125.41(5) 42_666 26_556
Ge4 Ba2 Ge4 125.41(6) 18_545 26_556
Ge4 Ba2 Ge4 125.41(6) 41_666 25_556
Ge4 Ba2 Ge4 61.1(3) 2 25_556
Ge4 Ba2 Ge4 80.85(9) . 25_556
Ge4 Ba2 Ge4 171.4(3) 42_666 25_556
Ge4 Ba2 Ge4 99.80(6) 18_545 25_556
Ge4 Ba2 Ge4 47.5(2) 26_556 25_556
Ge4 Ba2 Ge4 80.85(9) 41_666 17_545
Ge4 Ba2 Ge4 99.80(6) 2 17_545
Ge4 Ba2 Ge4 125.41(6) . 17_545
Ge4 Ba2 Ge4 61.1(3) 42_666 17_545
Ge4 Ba2 Ge4 47.5(2) 18_545 17_545
Ge4 Ba2 Ge4 171.4(3) 26_556 17_545
Ge4 Ba2 Ge4 125.41(6) 25_556 17_545
Ge4 Ba2 Ge3 5.09(8) 41_666 41_666
Ge4 Ba2 Ge3 166.3(2) 2 41_666
Ge4 Ba2 Ge3 120.74(4) . 41_666
Ge4 Ba2 Ge3 43.92(18) 42_666 41_666
Ge4 Ba2 Ge3 65.5(2) 18_545 41_666
Ge4 Ba2 Ge3 99.36(2) 26_556 41_666
Ge4 Ba2 Ge3 128.55(10) 25_556 41_666
Ge4 Ba2 Ge3 82.06(7) 17_545 41_666
Ge4 Ba2 Ge3 166.3(2) 41_666 2
Ge4 Ba2 Ge3 5.09(8) 2 2
Ge4 Ba2 Ge3 43.92(18) . 2
Ge4 Ba2 Ge3 120.74(4) 42_666 2
Ge4 Ba2 Ge3 128.55(10) 18_545 2
Ge4 Ba2 Ge3 82.06(7) 26_556 2
Ge4 Ba2 Ge3 65.5(2) 25_556 2
Ge4 Ba2 Ge3 99.36(2) 17_545 2
Ge3 Ba2 Ge3 161.31(19) 41_666 2
Ge4 Ba2 Ge3 43.92(18) 41_666 42_666
Ge4 Ba2 Ge3 128.55(10) 2 42_666
Ge4 Ba2 Ge3 99.36(2) . 42_666
Ge4 Ba2 Ge3 5.09(8) 42_666 42_666
Ge4 Ba2 Ge3 82.06(7) 18_545 42_666
Ge4 Ba2 Ge3 120.74(4) 26_556 42_666
Ge4 Ba2 Ge3 166.3(2) 25_556 42_666
Ge4 Ba2 Ge3 65.5(2) 17_545 42_666
Ge3 Ba2 Ge3 40.08(14) 41_666 42_666
Ge3 Ba2 Ge3 123.71(4) 2 42_666
Ge4 Ba2 Ge3 128.55(10) 41_666 .
Ge4 Ba2 Ge3 43.92(18) 2 .
Ge4 Ba2 Ge3 5.09(8) . .
Ge4 Ba2 Ge3 99.36(2) 42_666 .
Ge4 Ba2 Ge3 166.3(2) 18_545 .
Ge4 Ba2 Ge3 65.5(2) 26_556 .
Ge4 Ba2 Ge3 82.06(7) 25_556 .
Ge4 Ba2 Ge3 120.74(4) 17_545 .
Ge3 Ba2 Ge3 123.71(4) 41_666 .
Ge3 Ba2 Ge3 40.08(14) 2 .
Ge3 Ba2 Ge3 99.37(4) 42_666 .
Ge4 Ba2 Ge3 120.74(4) 41_666 25_556
Ge4 Ba2 Ge3 65.5(2) 2 25_556
Ge4 Ba2 Ge3 82.06(7) . 25_556
Ge4 Ba2 Ge3 166.3(2) 42_666 25_556
Ge4 Ba2 Ge3 99.36(2) 18_545 25_556
Ge4 Ba2 Ge3 43.92(18) 26_556 25_556
Ge4 Ba2 Ge3 5.09(8) 25_556 25_556
Ge4 Ba2 Ge3 128.55(10) 17_545 25_556
Ge3 Ba2 Ge3 123.71(4) 41_666 25_556
Ge3 Ba2 Ge3 69.82(16) 2 25_556
Ge3 Ba2 Ge3 161.31(19) 42_666 25_556
Ge3 Ba2 Ge3 83.68(7) . 25_556
Ge4 Ba2 Ge3 82.06(7) 41_666 17_545
Ge4 Ba2 Ge3 99.36(2) 2 17_545
Ge4 Ba2 Ge3 128.55(10) . 17_545
Ge4 Ba2 Ge3 65.5(2) 42_666 17_545
Ge4 Ba2 Ge3 43.92(18) 18_545 17_545
Ge4 Ba2 Ge3 166.3(2) 26_556 17_545
Ge4 Ba2 Ge3 120.74(4) 25_556 17_545
Ge4 Ba2 Ge3 5.09(8) 17_545 17_545
Ge3 Ba2 Ge3 83.68(7) 41_666 17_545
Ge3 Ba2 Ge3 99.37(4) 2 17_545
Ge3 Ba2 Ge3 69.82(16) 42_666 17_545
Ge3 Ba2 Ge3 123.71(4) . 17_545
Ge3 Ba2 Ge3 123.71(4) 25_556 17_545
Ge4 Ba2 Ge3 99.36(2) 41_666 26_556
Ge4 Ba2 Ge3 82.06(7) 2 26_556
Ge4 Ba2 Ge3 65.5(2) . 26_556
Ge4 Ba2 Ge3 128.55(10) 42_666 26_556
Ge4 Ba2 Ge3 120.74(4) 18_545 26_556
Ge4 Ba2 Ge3 5.09(8) 26_556 26_556
Ge4 Ba2 Ge3 43.92(18) 25_556 26_556
Ge4 Ba2 Ge3 166.3(2) 17_545 26_556
Ge3 Ba2 Ge3 99.37(4) 41_666 26_556
Ge3 Ba2 Ge3 83.68(7) 2 26_556
Ge3 Ba2 Ge3 123.71(4) 42_666 26_556
Ge3 Ba2 Ge3 69.82(16) . 26_556
Ge3 Ba2 Ge3 40.08(14) 25_556 26_556
Ge3 Ba2 Ge3 161.31(19) 17_545 26_556
Ge4 Ba2 Ge3 65.5(2) 41_666 18_545
Ge4 Ba2 Ge3 120.74(4) 2 18_545
Ge4 Ba2 Ge3 166.3(2) . 18_545
Ge4 Ba2 Ge3 82.06(7) 42_666 18_545
Ge4 Ba2 Ge3 5.09(8) 18_545 18_545
Ge4 Ba2 Ge3 128.55(10) 26_556 18_545
Ge4 Ba2 Ge3 99.36(2) 25_556 18_545
Ge4 Ba2 Ge3 43.92(18) 17_545 18_545
Ge3 Ba2 Ge3 69.82(16) 41_666 18_545
Ge3 Ba2 Ge3 123.71(4) 2 18_545
Ge3 Ba2 Ge3 83.68(7) 42_666 18_545
Ge3 Ba2 Ge3 161.31(19) . 18_545
Ge3 Ba2 Ge3 99.37(4) 25_556 18_545
Ge3 Ba2 Ge3 40.08(14) 17_545 18_545
Ge3 Ba2 Ge3 123.71(4) 26_556 18_545
Ge4 Ba2 Ge2 34.63(16) 41_666 33_656
Ge4 Ba2 Ge2 153.88(15) 2 33_656
Ge4 Ba2 Ge2 153.88(15) . 33_656
Ge4 Ba2 Ge2 75.30(7) 42_666 33_656
Ge4 Ba2 Ge2 34.63(16) 18_545 33_656
Ge4 Ba2 Ge2 100.29(10) 26_556 33_656
Ge4 Ba2 Ge2 100.29(10) 25_556 33_656
Ge4 Ba2 Ge2 75.30(7) 17_545 33_656
Ge3 Ba2 Ge2 39.73(9) 41_666 33_656
Ge3 Ba2 Ge2 158.67(9) 2 33_656
Ge3 Ba2 Ge2 73.47(4) 42_666 33_656
Ge3 Ba2 Ge2 158.67(9) . 33_656
Ge3 Ba2 Ge2 97.01(6) 25_556 33_656
Ge3 Ba2 Ge2 73.47(4) 17_545 33_656
Ge3 Ba2 Ge2 97.01(6) 26_556 33_656
Ge3 Ba2 Ge2 39.73(9) 18_545 33_656
Ge4 Ba2 Ge2 153.88(15) 41_666 29_556
Ge4 Ba2 Ge2 34.63(16) 2 29_556
Ge4 Ba2 Ge2 75.30(7) . 29_556
Ge4 Ba2 Ge2 153.88(15) 42_666 29_556
Ge4 Ba2 Ge2 100.29(10) 18_545 29_556
Ge4 Ba2 Ge2 75.30(7) 26_556 29_556
Ge4 Ba2 Ge2 34.63(16) 25_556 29_556
Ge4 Ba2 Ge2 100.29(10) 17_545 29_556
Ge3 Ba2 Ge2 158.67(9) 41_666 29_556
Ge3 Ba2 Ge2 39.73(9) 2 29_556
Ge3 Ba2 Ge2 158.67(9) 42_666 29_556
Ge3 Ba2 Ge2 73.47(4) . 29_556
Ge3 Ba2 Ge2 39.73(9) 25_556 29_556
Ge3 Ba2 Ge2 97.01(6) 17_545 29_556
Ge3 Ba2 Ge2 73.47(4) 26_556 29_556
Ge3 Ba2 Ge2 97.01(6) 18_545 29_556
Ge2 Ba2 Ge2 120.0 33_656 29_556
Ge4 Ba2 Rh1 34.63(16) 41_666 33_656
Ge4 Ba2 Rh1 153.88(15) 2 33_656
Ge4 Ba2 Rh1 153.88(15) . 33_656
Ge4 Ba2 Rh1 75.30(7) 42_666 33_656
Ge4 Ba2 Rh1 34.63(16) 18_545 33_656
Ge4 Ba2 Rh1 100.29(10) 26_556 33_656
Ge4 Ba2 Rh1 100.29(10) 25_556 33_656
Ge4 Ba2 Rh1 75.30(7) 17_545 33_656
Ge3 Ba2 Rh1 39.73(9) 41_666 33_656
Ge3 Ba2 Rh1 158.67(9) 2 33_656
Ge3 Ba2 Rh1 73.47(4) 42_666 33_656
Ge3 Ba2 Rh1 158.67(9) . 33_656
Ge3 Ba2 Rh1 97.01(6) 25_556 33_656
Ge3 Ba2 Rh1 73.47(4) 17_545 33_656
Ge3 Ba2 Rh1 97.01(6) 26_556 33_656
Ge3 Ba2 Rh1 39.73(9) 18_545 33_656
Ge2 Ba2 Rh1 0.0 33_656 33_656
Ge2 Ba2 Rh1 120.0 29_556 33_656
Ge4 Ba2 Rh1 153.88(15) 41_666 29_556
Ge4 Ba2 Rh1 34.63(16) 2 29_556
Ge4 Ba2 Rh1 75.30(7) . 29_556
Ge4 Ba2 Rh1 153.88(15) 42_666 29_556
Ge4 Ba2 Rh1 100.29(10) 18_545 29_556
Ge4 Ba2 Rh1 75.30(7) 26_556 29_556
Ge4 Ba2 Rh1 34.63(16) 25_556 29_556
Ge4 Ba2 Rh1 100.29(10) 17_545 29_556
Ge3 Ba2 Rh1 158.67(9) 41_666 29_556
Ge3 Ba2 Rh1 39.73(9) 2 29_556
Ge3 Ba2 Rh1 158.67(9) 42_666 29_556
Ge3 Ba2 Rh1 73.47(4) . 29_556
Ge3 Ba2 Rh1 39.73(9) 25_556 29_556
Ge3 Ba2 Rh1 97.01(6) 17_545 29_556
Ge3 Ba2 Rh1 73.47(4) 26_556 29_556
Ge3 Ba2 Rh1 97.01(6) 18_545 29_556
Ge2 Ba2 Rh1 120.0 33_656 29_556
Ge2 Ba2 Rh1 0.0 29_556 29_556
Rh1 Ba2 Rh1 120.0 33_656 29_556
Ge4 Ba2 Ge2 75.30(7) 41_666 9
Ge4 Ba2 Ge2 100.29(10) 2 9
Ge4 Ba2 Ge2 100.29(10) . 9
Ge4 Ba2 Ge2 34.63(16) 42_666 9
Ge4 Ba2 Ge2 75.30(7) 18_545 9
Ge4 Ba2 Ge2 153.88(15) 26_556 9
Ge4 Ba2 Ge2 153.88(15) 25_556 9
Ge4 Ba2 Ge2 34.63(16) 17_545 9
Ge3 Ba2 Ge2 73.47(4) 41_666 9
Ge3 Ba2 Ge2 97.01(6) 2 9
Ge3 Ba2 Ge2 39.73(9) 42_666 9
Ge3 Ba2 Ge2 97.01(6) . 9
Ge3 Ba2 Ge2 158.67(9) 25_556 9
Ge3 Ba2 Ge2 39.73(9) 17_545 9
Ge3 Ba2 Ge2 158.67(9) 26_556 9
Ge3 Ba2 Ge2 73.47(4) 18_545 9
Ge2 Ba2 Ge2 90.0 33_656 9
Ge2 Ba2 Ge2 120.0 29_556 9
Rh1 Ba2 Ge2 90.0 33_656 9
Rh1 Ba2 Ge2 120.0 29_556 9
Ge4 Ba2 Rh1 75.30(7) 41_666 9
Ge4 Ba2 Rh1 100.29(10) 2 9
Ge4 Ba2 Rh1 100.29(10) . 9
Ge4 Ba2 Rh1 34.63(16) 42_666 9
Ge4 Ba2 Rh1 75.30(7) 18_545 9
Ge4 Ba2 Rh1 153.88(15) 26_556 9
Ge4 Ba2 Rh1 153.88(15) 25_556 9
Ge4 Ba2 Rh1 34.63(16) 17_545 9
Ge3 Ba2 Rh1 73.47(4) 41_666 9
Ge3 Ba2 Rh1 97.01(6) 2 9
Ge3 Ba2 Rh1 39.73(9) 42_666 9
Ge3 Ba2 Rh1 97.01(6) . 9
Ge3 Ba2 Rh1 158.67(9) 25_556 9
Ge3 Ba2 Rh1 39.73(9) 17_545 9
Ge3 Ba2 Rh1 158.67(9) 26_556 9
Ge3 Ba2 Rh1 73.47(4) 18_545 9
Ge2 Ba2 Rh1 90.0 33_656 9
Ge2 Ba2 Rh1 120.0 29_556 9
Rh1 Ba2 Rh1 90.0 33_656 9
Rh1 Ba2 Rh1 120.0 29_556 9
Ge2 Ba2 Rh1 0.0 9 9
Ge4 Ba2 Ge2 100.29(10) 41_666 5
Ge4 Ba2 Ge2 75.30(7) 2 5
Ge4 Ba2 Ge2 34.63(16) . 5
Ge4 Ba2 Ge2 100.29(10) 42_666 5
Ge4 Ba2 Ge2 153.88(15) 18_545 5
Ge4 Ba2 Ge2 34.63(16) 26_556 5
Ge4 Ba2 Ge2 75.30(7) 25_556 5
Ge4 Ba2 Ge2 153.88(15) 17_545 5
Ge3 Ba2 Ge2 97.01(6) 41_666 5
Ge3 Ba2 Ge2 73.47(4) 2 5
Ge3 Ba2 Ge2 97.01(6) 42_666 5
Ge3 Ba2 Ge2 39.73(9) . 5
Ge3 Ba2 Ge2 73.47(4) 25_556 5
Ge3 Ba2 Ge2 158.67(9) 17_545 5
Ge3 Ba2 Ge2 39.73(9) 26_556 5
Ge3 Ba2 Ge2 158.67(9) 18_545 5
Ge2 Ba2 Ge2 120.0 33_656 5
Ge2 Ba2 Ge2 90.0 29_556 5
Rh1 Ba2 Ge2 120.0 33_656 5
Rh1 Ba2 Ge2 90.0 29_556 5
Ge2 Ba2 Ge2 120.0 9 5
Rh1 Ba2 Ge2 120.0 9 5
Ge4 Ba2 Rh1 100.29(10) 41_666 5
Ge4 Ba2 Rh1 75.30(7) 2 5
Ge4 Ba2 Rh1 34.63(16) . 5
Ge4 Ba2 Rh1 100.29(10) 42_666 5
Ge4 Ba2 Rh1 153.88(15) 18_545 5
Ge4 Ba2 Rh1 34.63(16) 26_556 5
Ge4 Ba2 Rh1 75.30(7) 25_556 5
Ge4 Ba2 Rh1 153.88(15) 17_545 5
Ge3 Ba2 Rh1 97.01(6) 41_666 5
Ge3 Ba2 Rh1 73.47(4) 2 5
Ge3 Ba2 Rh1 97.01(6) 42_666 5
Ge3 Ba2 Rh1 39.73(9) . 5
Ge3 Ba2 Rh1 73.47(4) 25_556 5
Ge3 Ba2 Rh1 158.67(9) 17_545 5
Ge3 Ba2 Rh1 39.73(9) 26_556 5
Ge3 Ba2 Rh1 158.67(9) 18_545 5
Ge2 Ba2 Rh1 120.0 33_656 5
Ge2 Ba2 Rh1 90.0 29_556 5
Rh1 Ba2 Rh1 120.0 33_656 5
Rh1 Ba2 Rh1 90.0 29_556 5
Ge2 Ba2 Rh1 120.0 9 5
Rh1 Ba2 Rh1 120.0 9 5
Ge2 Ba2 Rh1 0.0 5 5
Ge4 Ba2 Ge1 39.88(7) 41_666 37_666
Ge4 Ba2 Ge1 136.84(6) 2 37_666
Ge4 Ba2 Ge1 92.56(14) . 37_666
Ge4 Ba2 Ge1 68.28(16) 42_666 37_666
Ge4 Ba2 Ge1 95.63(16) 18_545 37_666
Ge4 Ba2 Ge1 62.77(4) 26_556 37_666
Ge4 Ba2 Ge1 103.13(15) 25_556 37_666
Ge4 Ba2 Ge1 119.71(7) 17_545 37_666
Ge3 Ba2 Ge1 37.88(4) 41_666 37_666
Ge3 Ba2 Ge1 135.02(4) 2 37_666
Ge3 Ba2 Ge1 63.20(9) 42_666 37_666
Ge3 Ba2 Ge1 97.13(9) . 37_666
Ge3 Ba2 Ge1 98.16(9) 25_556 37_666
Ge3 Ba2 Ge1 121.55(4) 17_545 37_666
Ge3 Ba2 Ge1 63.82(3) 26_556 37_666
Ge3 Ba2 Ge1 100.65(9) 18_545 37_666
Ge2 Ba2 Ge1 61.609(2) 33_656 37_666
Ge2 Ba2 Ge1 136.721(9) 29_556 37_666
Rh1 Ba2 Ge1 61.609(2) 33_656 37_666
Rh1 Ba2 Ge1 136.721(9) 29_556 37_666
Ge2 Ba2 Ge1 102.882(10) 9 37_666
Rh1 Ba2 Ge1 102.882(10) 9 37_666
Ge2 Ba2 Ge1 61.609(2) 5 37_666
Rh1 Ba2 Ge1 61.609(2) 5 37_666
Ge4 Ba2 Ge1 136.84(6) 41_666 27
Ge4 Ba2 Ge1 39.88(7) 2 27
Ge4 Ba2 Ge1 68.28(16) . 27
Ge4 Ba2 Ge1 92.56(14) 42_666 27
Ge4 Ba2 Ge1 103.13(15) 18_545 27
Ge4 Ba2 Ge1 119.71(7) 26_556 27
Ge4 Ba2 Ge1 95.63(16) 25_556 27
Ge4 Ba2 Ge1 62.77(4) 17_545 27
Ge3 Ba2 Ge1 135.02(4) 41_666 27
Ge3 Ba2 Ge1 37.88(4) 2 27
Ge3 Ba2 Ge1 97.13(9) 42_666 27
Ge3 Ba2 Ge1 63.20(9) . 27
Ge3 Ba2 Ge1 100.65(9) 25_556 27
Ge3 Ba2 Ge1 63.82(3) 17_545 27
Ge3 Ba2 Ge1 121.55(4) 26_556 27
Ge3 Ba2 Ge1 98.16(9) 18_545 27
Ge2 Ba2 Ge1 136.721(9) 33_656 27
Ge2 Ba2 Ge1 61.609(2) 29_556 27
Rh1 Ba2 Ge1 136.721(9) 33_656 27
Rh1 Ba2 Ge1 61.609(2) 29_556 27
Ge2 Ba2 Ge1 61.609(2) 9 27
Rh1 Ba2 Ge1 61.609(2) 9 27
Ge2 Ba2 Ge1 102.882(10) 5 27
Rh1 Ba2 Ge1 102.882(10) 5 27
Ge1 Ba2 Ge1 150.744(16) 37_666 27
Ge4 Ba2 Ge1 119.71(7) 41_666 39_656
Ge4 Ba2 Ge1 62.77(4) 2 39_656
Ge4 Ba2 Ge1 103.13(15) . 39_656
Ge4 Ba2 Ge1 95.63(16) 42_666 39_656
Ge4 Ba2 Ge1 68.28(16) 18_545 39_656
Ge4 Ba2 Ge1 136.84(6) 26_556 39_656
Ge4 Ba2 Ge1 92.56(14) 25_556 39_656
Ge4 Ba2 Ge1 39.88(7) 17_545 39_656
Ge3 Ba2 Ge1 121.55(4) 41_666 39_656
Ge3 Ba2 Ge1 63.82(3) 2 39_656
Ge3 Ba2 Ge1 100.65(9) 42_666 39_656
Ge3 Ba2 Ge1 98.16(9) . 39_656
Ge3 Ba2 Ge1 97.13(9) 25_556 39_656
Ge3 Ba2 Ge1 37.88(4) 17_545 39_656
Ge3 Ba2 Ge1 135.02(4) 26_556 39_656
Ge3 Ba2 Ge1 63.20(9) 18_545 39_656
Ge2 Ba2 Ge1 102.882(10) 33_656 39_656
Ge2 Ba2 Ge1 61.609(2) 29_556 39_656
Rh1 Ba2 Ge1 102.882(10) 33_656 39_656
Rh1 Ba2 Ge1 61.609(2) 29_556 39_656
Ge2 Ba2 Ge1 61.609(2) 9 39_656
Rh1 Ba2 Ge1 61.609(2) 9 39_656
Ge2 Ba2 Ge1 136.721(9) 5 39_656
Rh1 Ba2 Ge1 136.721(9) 5 39_656
Ge1 Ba2 Ge1 159.426(11) 37_666 39_656
Ge1 Ba2 Ge1 36.03(2) 27 39_656
Ge4 Ba2 Ge1 62.77(4) 41_666 26_556
Ge4 Ba2 Ge1 119.71(7) 2 26_556
Ge4 Ba2 Ge1 95.63(16) . 26_556
Ge4 Ba2 Ge1 103.13(15) 42_666 26_556
Ge4 Ba2 Ge1 92.56(14) 18_545 26_556
Ge4 Ba2 Ge1 39.88(7) 26_556 26_556
Ge4 Ba2 Ge1 68.28(16) 25_556 26_556
Ge4 Ba2 Ge1 136.84(6) 17_545 26_556
Ge3 Ba2 Ge1 63.82(3) 41_666 26_556
Ge3 Ba2 Ge1 121.55(4) 2 26_556
Ge3 Ba2 Ge1 98.16(9) 42_666 26_556
Ge3 Ba2 Ge1 100.65(9) . 26_556
Ge3 Ba2 Ge1 63.20(10) 25_556 26_556
Ge3 Ba2 Ge1 135.02(4) 17_545 26_556
Ge3 Ba2 Ge1 37.88(4) 26_556 26_556
Ge3 Ba2 Ge1 97.13(9) 18_545 26_556
Ge2 Ba2 Ge1 61.609(2) 33_656 26_556
Ge2 Ba2 Ge1 102.882(10) 29_556 26_556
Rh1 Ba2 Ge1 61.609(2) 33_656 26_556
Rh1 Ba2 Ge1 102.882(10) 29_556 26_556
Ge2 Ba2 Ge1 136.721(9) 9 26_556
Rh1 Ba2 Ge1 136.721(9) 9 26_556
Ge2 Ba2 Ge1 61.609(2) 5 26_556
Rh1 Ba2 Ge1 61.609(2) 5 26_556
Ge1 Ba2 Ge1 36.03(2) 37_666 26_556
Ge1 Ba2 Ge1 159.426(11) 27 26_556
Ge1 Ba2 Ge1 150.744(16) 39_656 26_556
Ge4 Ba2 Ge1 68.28(16) 41_666 14
Ge4 Ba2 Ge1 103.13(15) 2 14
Ge4 Ba2 Ge1 62.77(4) . 14
Ge4 Ba2 Ge1 39.88(7) 42_666 14
Ge4 Ba2 Ge1 119.71(7) 18_545 14
Ge4 Ba2 Ge1 92.56(14) 26_556 14
Ge4 Ba2 Ge1 136.84(6) 25_556 14
Ge4 Ba2 Ge1 95.63(16) 17_545 14
Ge3 Ba2 Ge1 63.20(9) 41_666 14
Ge3 Ba2 Ge1 98.16(9) 2 14
Ge3 Ba2 Ge1 37.88(4) 42_666 14
Ge3 Ba2 Ge1 63.82(3) . 14
Ge3 Ba2 Ge1 135.02(4) 25_556 14
Ge3 Ba2 Ge1 100.65(9) 17_545 14
Ge3 Ba2 Ge1 97.13(9) 26_556 14
Ge3 Ba2 Ge1 121.55(4) 18_545 14
Ge2 Ba2 Ge1 102.882(10) 33_656 14
Ge2 Ba2 Ge1 136.721(9) 29_556 14
Rh1 Ba2 Ge1 102.882(10) 33_656 14
Rh1 Ba2 Ge1 136.721(9) 29_556 14
Ge2 Ba2 Ge1 61.609(2) 9 14
Rh1 Ba2 Ge1 61.609(2) 9 14
Ge2 Ba2 Ge1 61.609(2) 5 14
Rh1 Ba2 Ge1 61.609(2) 5 14
Ge1 Ba2 Ge1 59.189(18) 37_666 14
Ge1 Ba2 Ge1 91.827(2) 27 14
Ge1 Ba2 Ge1 116.643(13) 39_656 14
Ge1 Ba2 Ge1 91.827(2) 26_556 14
Ge4 Ba2 Ge1 103.13(15) 41_666 .
Ge4 Ba2 Ge1 68.28(16) 2 .
Ge4 Ba2 Ge1 39.88(7) . .
Ge4 Ba2 Ge1 62.77(4) 42_666 .
Ge4 Ba2 Ge1 136.84(6) 18_545 .
Ge4 Ba2 Ge1 95.63(16) 26_556 .
Ge4 Ba2 Ge1 119.71(7) 25_556 .
Ge4 Ba2 Ge1 92.56(14) 17_545 .
Ge3 Ba2 Ge1 98.16(9) 41_666 .
Ge3 Ba2 Ge1 63.20(9) 2 .
Ge3 Ba2 Ge1 63.82(3) 42_666 .
Ge3 Ba2 Ge1 37.88(4) . .
Ge3 Ba2 Ge1 121.55(4) 25_556 .
Ge3 Ba2 Ge1 97.13(9) 17_545 .
Ge3 Ba2 Ge1 100.65(9) 26_556 .
Ge3 Ba2 Ge1 135.02(4) 18_545 .
Ge2 Ba2 Ge1 136.721(9) 33_656 .
Ge2 Ba2 Ge1 102.882(10) 29_556 .
Rh1 Ba2 Ge1 136.721(9) 33_656 .
Rh1 Ba2 Ge1 102.882(10) 29_556 .
Ge2 Ba2 Ge1 61.609(2) 9 .
Rh1 Ba2 Ge1 61.609(2) 9 .
Ge2 Ba2 Ge1 61.609(2) 5 .
Rh1 Ba2 Ge1 61.609(2) 5 .
Ge1 Ba2 Ge1 91.827(2) 37_666 .
Ge1 Ba2 Ge1 59.189(18) 27 .
Ge1 Ba2 Ge1 91.827(2) 39_656 .
Ge1 Ba2 Ge1 116.643(13) 26_556 .
Ge1 Ba2 Ge1 36.03(2) 14 .
Ge4 Ba2 Ge1 95.63(16) 41_666 16_545
Ge4 Ba2 Ge1 92.56(14) 2 16_545
Ge4 Ba2 Ge1 136.84(6) . 16_545
Ge4 Ba2 Ge1 119.71(7) 42_666 16_545
Ge4 Ba2 Ge1 39.88(7) 18_545 16_545
Ge4 Ba2 Ge1 103.13(15) 26_556 16_545
Ge4 Ba2 Ge1 62.77(4) 25_556 16_545
Ge4 Ba2 Ge1 68.28(16) 17_545 16_545
Ge3 Ba2 Ge1 100.65(9) 41_666 16_545
Ge3 Ba2 Ge1 97.13(9) 2 16_545
Ge3 Ba2 Ge1 121.55(4) 42_666 16_545
Ge3 Ba2 Ge1 135.02(4) . 16_545
Ge3 Ba2 Ge1 63.82(3) 25_556 16_545
Ge3 Ba2 Ge1 63.20(9) 17_545 16_545
Ge3 Ba2 Ge1 98.16(9) 26_556 16_545
Ge3 Ba2 Ge1 37.88(4) 18_545 16_545
Ge2 Ba2 Ge1 61.609(2) 33_656 16_545
Ge2 Ba2 Ge1 61.609(2) 29_556 16_545
Rh1 Ba2 Ge1 61.609(2) 33_656 16_545
Rh1 Ba2 Ge1 61.609(2) 29_556 16_545
Ge2 Ba2 Ge1 102.882(10) 9 16_545
Rh1 Ba2 Ge1 102.882(10) 9 16_545
Ge2 Ba2 Ge1 136.721(9) 5 16_545
Rh1 Ba2 Ge1 136.721(9) 5 16_545
Ge1 Ba2 Ge1 116.643(13) 37_666 16_545
Ge1 Ba2 Ge1 91.827(2) 27 16_545
Ge1 Ba2 Ge1 59.189(18) 39_656 16_545
Ge1 Ba2 Ge1 91.827(2) 26_556 16_545
Ge1 Ba2 Ge1 159.426(11) 14 16_545
Ge1 Ba2 Ge1 150.744(16) . 16_545
Ge4 Ba2 Ge1 92.56(14) 41_666 4_556
Ge4 Ba2 Ge1 95.63(16) 2 4_556
Ge4 Ba2 Ge1 119.71(7) . 4_556
Ge4 Ba2 Ge1 136.84(6) 42_666 4_556
Ge4 Ba2 Ge1 62.77(4) 18_545 4_556
Ge4 Ba2 Ge1 68.28(16) 26_556 4_556
Ge4 Ba2 Ge1 39.88(7) 25_556 4_556
Ge4 Ba2 Ge1 103.13(15) 17_545 4_556
Ge3 Ba2 Ge1 97.13(9) 41_666 4_556
Ge3 Ba2 Ge1 100.65(9) 2 4_556
Ge3 Ba2 Ge1 135.02(4) 42_666 4_556
Ge3 Ba2 Ge1 121.55(4) . 4_556
Ge3 Ba2 Ge1 37.88(4) 25_556 4_556
Ge3 Ba2 Ge1 98.16(9) 17_545 4_556
Ge3 Ba2 Ge1 63.20(9) 26_556 4_556
Ge3 Ba2 Ge1 63.82(3) 18_545 4_556
Ge2 Ba2 Ge1 61.609(2) 33_656 4_556
Ge2 Ba2 Ge1 61.609(2) 29_556 4_556
Rh1 Ba2 Ge1 61.609(2) 33_656 4_556
Rh1 Ba2 Ge1 61.609(2) 29_556 4_556
Ge2 Ba2 Ge1 136.721(9) 9 4_556
Rh1 Ba2 Ge1 136.721(9) 9 4_556
Ge2 Ba2 Ge1 102.882(10) 5 4_556
Rh1 Ba2 Ge1 102.882(10) 5 4_556
Ge1 Ba2 Ge1 91.827(2) 37_666 4_556
Ge1 Ba2 Ge1 116.643(13) 27 4_556
Ge1 Ba2 Ge1 91.827(2) 39_656 4_556
Ge1 Ba2 Ge1 59.189(18) 26_556 4_556
Ge1 Ba2 Ge1 150.744(16) 14 4_556
Ge1 Ba2 Ge1 159.426(11) . 4_556
Ge1 Ba2 Ge1 36.03(2) 16_545 4_556
Ge4 Ba2 Ge4 131.57(4) 41_666 46_656
Ge4 Ba2 Ge4 55.9(2) 2 46_656
Ge4 Ba2 Ge4 103.00(4) . 46_656
Ge4 Ba2 Ge4 131.57(4) 42_666 46_656
Ge4 Ba2 Ge4 70.8(2) 18_545 46_656
Ge4 Ba2 Ge4 103.00(4) 26_556 46_656
Ge4 Ba2 Ge4 55.9(2) 25_556 46_656
Ge4 Ba2 Ge4 70.8(2) 17_545 46_656
Ge3 Ba2 Ge4 136.24(5) 41_666 46_656
Ge3 Ba2 Ge4 60.12(17) 2 46_656
Ge3 Ba2 Ge4 136.24(5) 42_666 46_656
Ge3 Ba2 Ge4 99.81(6) . 46_656
Ge3 Ba2 Ge4 60.12(17) 25_556 46_656
Ge3 Ba2 Ge4 66.78(19) 17_545 46_656
Ge3 Ba2 Ge4 99.81(6) 26_556 46_656
Ge3 Ba2 Ge4 66.78(19) 18_545 46_656
Ge2 Ba2 Ge4 98.95(9) 33_656 46_656
Ge2 Ba2 Ge4 32.29(13) 29_556 46_656
Rh1 Ba2 Ge4 98.95(9) 33_656 46_656
Rh1 Ba2 Ge4 32.29(13) 29_556 46_656
Ge2 Ba2 Ge4 98.95(9) 9 46_656
Rh1 Ba2 Ge4 98.95(9) 9 46_656
Ge2 Ba2 Ge4 122.29(13) 5 46_656
Rh1 Ba2 Ge4 122.29(13) 5 46_656
Ge1 Ba2 Ge4 150.394(10) 37_666 46_656
Ge1 Ba2 Ge4 58.597(13) 27 46_656
Ge1 Ba2 Ge4 37.74(8) 39_656 46_656
Ge1 Ba2 Ge4 116.26(4) 26_556 46_656
Ge1 Ba2 Ge4 150.394(10) 14 46_656
Ge1 Ba2 Ge4 116.26(4) . 46_656
Ge1 Ba2 Ge4 37.74(8) 16_545 46_656
Ge1 Ba2 Ge4 58.597(13) 4_556 46_656
Ge4 Ba2 Ge4 55.9(2) 41_666 6_556
Ge4 Ba2 Ge4 131.57(4) 2 6_556
Ge4 Ba2 Ge4 131.57(4) . 6_556
Ge4 Ba2 Ge4 103.00(4) 42_666 6_556
Ge4 Ba2 Ge4 55.9(2) 18_545 6_556
Ge4 Ba2 Ge4 70.8(2) 26_556 6_556
Ge4 Ba2 Ge4 70.8(2) 25_556 6_556
Ge4 Ba2 Ge4 103.00(4) 17_545 6_556
Ge3 Ba2 Ge4 60.12(17) 41_666 6_556
Ge3 Ba2 Ge4 136.24(5) 2 6_556
Ge3 Ba2 Ge4 99.81(6) 42_666 6_556
Ge3 Ba2 Ge4 136.24(5) . 6_556
Ge3 Ba2 Ge4 66.78(19) 25_556 6_556
Ge3 Ba2 Ge4 99.81(6) 17_545 6_556
Ge3 Ba2 Ge4 66.78(19) 26_556 6_556
Ge3 Ba2 Ge4 60.12(17) 18_545 6_556
Ge2 Ba2 Ge4 32.29(13) 33_656 6_556
Ge2 Ba2 Ge4 98.95(9) 29_556 6_556
Rh1 Ba2 Ge4 32.29(13) 33_656 6_556
Rh1 Ba2 Ge4 98.95(9) 29_556 6_556
Ge2 Ba2 Ge4 122.29(13) 9 6_556
Rh1 Ba2 Ge4 122.29(13) 9 6_556
Ge2 Ba2 Ge4 98.95(9) 5 6_556
Rh1 Ba2 Ge4 98.95(9) 5 6_556
Ge1 Ba2 Ge4 58.597(13) 37_666 6_556
Ge1 Ba2 Ge4 150.394(10) 27 6_556
Ge1 Ba2 Ge4 116.26(4) 39_656 6_556
Ge1 Ba2 Ge4 37.74(8) 26_556 6_556
Ge1 Ba2 Ge4 116.26(4) 14 6_556
Ge1 Ba2 Ge4 150.394(10) . 6_556
Ge1 Ba2 Ge4 58.597(13) 16_545 6_556
Ge1 Ba2 Ge4 37.74(8) 4_556 6_556
Ge4 Ba2 Ge4 92.78(6) 46_656 6_556
Ge4 Ba2 Ge4 70.8(2) 41_666 45_666
Ge4 Ba2 Ge4 103.00(4) 2 45_666
Ge4 Ba2 Ge4 55.9(2) . 45_666
Ge4 Ba2 Ge4 70.8(2) 42_666 45_666
Ge4 Ba2 Ge4 131.57(4) 18_545 45_666
Ge4 Ba2 Ge4 55.9(2) 26_556 45_666
Ge4 Ba2 Ge4 103.00(4) 25_556 45_666
Ge4 Ba2 Ge4 131.57(4) 17_545 45_666
Ge3 Ba2 Ge4 66.78(19) 41_666 45_666
Ge3 Ba2 Ge4 99.81(6) 2 45_666
Ge3 Ba2 Ge4 66.78(19) 42_666 45_666
Ge3 Ba2 Ge4 60.12(17) . 45_666
Ge3 Ba2 Ge4 99.81(6) 25_556 45_666
Ge3 Ba2 Ge4 136.24(5) 17_545 45_666
Ge3 Ba2 Ge4 60.12(17) 26_556 45_666
Ge3 Ba2 Ge4 136.24(5) 18_545 45_666
Ge2 Ba2 Ge4 98.95(9) 33_656 45_666
Ge2 Ba2 Ge4 122.29(13) 29_556 45_666
Rh1 Ba2 Ge4 98.95(9) 33_656 45_666
Rh1 Ba2 Ge4 122.29(13) 29_556 45_666
Ge2 Ba2 Ge4 98.95(9) 9 45_666
Rh1 Ba2 Ge4 98.95(9) 9 45_666
Ge2 Ba2 Ge4 32.29(13) 5 45_666
Rh1 Ba2 Ge4 32.29(13) 5 45_666
Ge1 Ba2 Ge4 37.74(8) 37_666 45_666
Ge1 Ba2 Ge4 116.26(4) 27 45_666
Ge1 Ba2 Ge4 150.394(10) 39_656 45_666
Ge1 Ba2 Ge4 58.597(13) 26_556 45_666
Ge1 Ba2 Ge4 37.74(8) 14 45_666
Ge1 Ba2 Ge4 58.597(13) . 45_666
Ge1 Ba2 Ge4 150.394(10) 16_545 45_666
Ge1 Ba2 Ge4 116.26(4) 4_556 45_666
Ge4 Ba2 Ge4 154.6(3) 46_656 45_666
Ge4 Ba2 Ge4 92.78(6) 6_556 45_666
Ge4 Ba2 Ge4 103.00(4) 41_666 5
Ge4 Ba2 Ge4 70.8(2) 2 5
Ge4 Ba2 Ge4 70.8(2) . 5
Ge4 Ba2 Ge4 55.9(2) 42_666 5
Ge4 Ba2 Ge4 103.00(4) 18_545 5
Ge4 Ba2 Ge4 131.57(4) 26_556 5
Ge4 Ba2 Ge4 131.57(4) 25_556 5
Ge4 Ba2 Ge4 55.9(2) 17_545 5
Ge3 Ba2 Ge4 99.81(6) 41_666 5
Ge3 Ba2 Ge4 66.78(19) 2 5
Ge3 Ba2 Ge4 60.12(17) 42_666 5
Ge3 Ba2 Ge4 66.78(19) . 5
Ge3 Ba2 Ge4 136.24(5) 25_556 5
Ge3 Ba2 Ge4 60.12(17) 17_545 5
Ge3 Ba2 Ge4 136.24(5) 26_556 5
Ge3 Ba2 Ge4 99.81(6) 18_545 5
Ge2 Ba2 Ge4 122.29(13) 33_656 5
Ge2 Ba2 Ge4 98.95(9) 29_556 5
Rh1 Ba2 Ge4 122.29(13) 33_656 5
Rh1 Ba2 Ge4 98.95(9) 29_556 5
Ge2 Ba2 Ge4 32.29(13) 9 5
Rh1 Ba2 Ge4 32.29(13) 9 5
Ge2 Ba2 Ge4 98.95(9) 5 5
Rh1 Ba2 Ge4 98.95(9) 5 5
Ge1 Ba2 Ge4 116.26(4) 37_666 5
Ge1 Ba2 Ge4 37.74(8) 27 5
Ge1 Ba2 Ge4 58.597(13) 39_656 5
Ge1 Ba2 Ge4 150.394(10) 26_556 5
Ge1 Ba2 Ge4 58.597(13) 14 5
Ge1 Ba2 Ge4 37.74(8) . 5
Ge1 Ba2 Ge4 116.26(4) 16_545 5
Ge1 Ba2 Ge4 150.394(10) 4_556 5
Ge4 Ba2 Ge4 92.78(6) 46_656 5
Ge4 Ba2 Ge4 154.6(3) 6_556 5
Ge4 Ba2 Ge4 92.78(6) 45_666 5
Ge4 Ba2 Ge3 67.07(20) 41_666 45_666
Ge4 Ba2 Ge3 106.53(5) 2 45_666
Ge4 Ba2 Ge3 59.26(18) . 45_666
Ge4 Ba2 Ge3 67.1(2) 42_666 45_666
Ge4 Ba2 Ge3 128.04(9) 18_545 45_666
Ge4 Ba2 Ge3 59.26(18) 26_556 45_666
Ge4 Ba2 Ge3 106.53(5) 25_556 45_666
Ge4 Ba2 Ge3 128.04(9) 17_545 45_666
Ge3 Ba2 Ge3 62.93(15) 41_666 45_666
Ge3 Ba2 Ge3 103.18(2) 2 45_666
Ge3 Ba2 Ge3 62.93(15) 42_666 45_666
Ge3 Ba2 Ge3 63.27(13) . 45_666
Ge3 Ba2 Ge3 103.18(2) 25_556 45_666
Ge3 Ba2 Ge3 132.596(16) 17_545 45_666
Ge3 Ba2 Ge3 63.27(13) 26_556 45_666
Ge3 Ba2 Ge3 132.596(16) 18_545 45_666
Ge2 Ba2 Ge3 96.04(5) 33_656 45_666
Ge2 Ba2 Ge3 126.44(8) 29_556 45_666
Rh1 Ba2 Ge3 96.04(5) 33_656 45_666
Rh1 Ba2 Ge3 126.44(8) 29_556 45_666
Ge2 Ba2 Ge3 96.04(5) 9 45_666
Rh1 Ba2 Ge3 96.04(5) 9 45_666
Ge2 Ba2 Ge3 36.44(8) 5 45_666
Rh1 Ba2 Ge3 36.44(8) 5 45_666
Ge1 Ba2 Ge3 35.42(4) 37_666 45_666
Ge1 Ba2 Ge3 117.50(2) 27 45_666
Ge1 Ba2 Ge3 150.240(11) 39_656 45_666
Ge1 Ba2 Ge3 59.007(12) 26_556 45_666
Ge1 Ba2 Ge3 35.42(4) 14 45_666
Ge1 Ba2 Ge3 59.007(12) . 45_666
Ge1 Ba2 Ge3 150.240(11) 16_545 45_666
Ge1 Ba2 Ge3 117.50(2) 4_556 45_666
Ge4 Ba2 Ge3 158.7(2) 46_656 45_666
Ge4 Ba2 Ge3 91.88(4) 6_556 45_666
Ge4 Ba2 Ge3 4.15(7) 45_666 45_666
Ge4 Ba2 Ge3 91.88(4) 5 45_666
Ge4 Ba2 Ge3 106.53(5) 41_666 5
Ge4 Ba2 Ge3 67.07(19) 2 5
Ge4 Ba2 Ge3 67.07(19) . 5
Ge4 Ba2 Ge3 59.26(18) 42_666 5
Ge4 Ba2 Ge3 106.53(5) 18_545 5
Ge4 Ba2 Ge3 128.04(9) 26_556 5
Ge4 Ba2 Ge3 128.04(9) 25_556 5
Ge4 Ba2 Ge3 59.26(18) 17_545 5
Ge3 Ba2 Ge3 103.18(2) 41_666 5
Ge3 Ba2 Ge3 62.93(15) 2 5
Ge3 Ba2 Ge3 63.27(13) 42_666 5
Ge3 Ba2 Ge3 62.93(15) . 5
Ge3 Ba2 Ge3 132.596(16) 25_556 5
Ge3 Ba2 Ge3 63.27(13) 17_545 5
Ge3 Ba2 Ge3 132.596(16) 26_556 5
Ge3 Ba2 Ge3 103.18(2) 18_545 5
Ge2 Ba2 Ge3 126.44(8) 33_656 5
Ge2 Ba2 Ge3 96.04(5) 29_556 5
Rh1 Ba2 Ge3 126.44(8) 33_656 5
Rh1 Ba2 Ge3 96.04(5) 29_556 5
Ge2 Ba2 Ge3 36.44(8) 9 5
Rh1 Ba2 Ge3 36.44(8) 9 5
Ge2 Ba2 Ge3 96.04(5) 5 5
Rh1 Ba2 Ge3 96.04(5) 5 5
Ge1 Ba2 Ge3 117.50(2) 37_666 5
Ge1 Ba2 Ge3 35.42(4) 27 5
Ge1 Ba2 Ge3 59.007(12) 39_656 5
Ge1 Ba2 Ge3 150.240(11) 26_556 5
Ge1 Ba2 Ge3 59.007(12) 14 5
Ge1 Ba2 Ge3 35.42(4) . 5
Ge1 Ba2 Ge3 117.50(2) 16_545 5
Ge1 Ba2 Ge3 150.240(11) 4_556 5
Ge4 Ba2 Ge3 91.88(4) 46_656 5
Ge4 Ba2 Ge3 158.7(2) 6_556 5
Ge4 Ba2 Ge3 91.88(4) 45_666 5
Ge4 Ba2 Ge3 4.15(7) 5 5
Ge3 Ba2 Ge3 91.27(2) 45_666 5
Ge4 Ba2 Ge3 128.04(9) 41_666 46_656
Ge4 Ba2 Ge3 59.26(18) 2 46_656
Ge4 Ba2 Ge3 106.53(5) . 46_656
Ge4 Ba2 Ge3 128.04(9) 42_666 46_656
Ge4 Ba2 Ge3 67.1(2) 18_545 46_656
Ge4 Ba2 Ge3 106.53(5) 26_556 46_656
Ge4 Ba2 Ge3 59.26(18) 25_556 46_656
Ge4 Ba2 Ge3 67.1(2) 17_545 46_656
Ge3 Ba2 Ge3 132.596(17) 41_666 46_656
Ge3 Ba2 Ge3 63.27(13) 2 46_656
Ge3 Ba2 Ge3 132.596(17) 42_666 46_656
Ge3 Ba2 Ge3 103.18(2) . 46_656
Ge3 Ba2 Ge3 63.27(13) 25_556 46_656
Ge3 Ba2 Ge3 62.93(15) 17_545 46_656
Ge3 Ba2 Ge3 103.18(2) 26_556 46_656
Ge3 Ba2 Ge3 62.93(15) 18_545 46_656
Ge2 Ba2 Ge3 96.04(5) 33_656 46_656
Ge2 Ba2 Ge3 36.44(8) 29_556 46_656
Rh1 Ba2 Ge3 96.04(5) 33_656 46_656
Rh1 Ba2 Ge3 36.44(8) 29_556 46_656
Ge2 Ba2 Ge3 96.04(5) 9 46_656
Rh1 Ba2 Ge3 96.04(5) 9 46_656
Ge2 Ba2 Ge3 126.44(8) 5 46_656
Rh1 Ba2 Ge3 126.44(8) 5 46_656
Ge1 Ba2 Ge3 150.240(11) 37_666 46_656
Ge1 Ba2 Ge3 59.007(13) 27 46_656
Ge1 Ba2 Ge3 35.42(4) 39_656 46_656
Ge1 Ba2 Ge3 117.50(2) 26_556 46_656
Ge1 Ba2 Ge3 150.240(11) 14 46_656
Ge1 Ba2 Ge3 117.50(2) . 46_656
Ge1 Ba2 Ge3 35.42(4) 16_545 46_656
Ge1 Ba2 Ge3 59.007(12) 4_556 46_656
Ge4 Ba2 Ge3 4.15(7) 46_656 46_656
Ge4 Ba2 Ge3 91.88(4) 6_556 46_656
Ge4 Ba2 Ge3 158.7(2) 45_666 46_656
Ge4 Ba2 Ge3 91.88(4) 5 46_656
Ge3 Ba2 Ge3 162.88(15) 45_666 46_656
Ge3 Ba2 Ge3 91.27(2) 5 46_656
Ge4 Ba2 Ge3 59.26(18) 41_666 6_556
Ge4 Ba2 Ge3 128.04(9) 2 6_556
Ge4 Ba2 Ge3 128.04(9) . 6_556
Ge4 Ba2 Ge3 106.53(5) 42_666 6_556
Ge4 Ba2 Ge3 59.26(18) 18_545 6_556
Ge4 Ba2 Ge3 67.07(19) 26_556 6_556
Ge4 Ba2 Ge3 67.1(2) 25_556 6_556
Ge4 Ba2 Ge3 106.53(5) 17_545 6_556
Ge3 Ba2 Ge3 63.27(13) 41_666 6_556
Ge3 Ba2 Ge3 132.596(16) 2 6_556
Ge3 Ba2 Ge3 103.18(2) 42_666 6_556
Ge3 Ba2 Ge3 132.596(16) . 6_556
Ge3 Ba2 Ge3 62.93(15) 25_556 6_556
Ge3 Ba2 Ge3 103.18(2) 17_545 6_556
Ge3 Ba2 Ge3 62.93(15) 26_556 6_556
Ge3 Ba2 Ge3 63.27(13) 18_545 6_556
Ge2 Ba2 Ge3 36.44(8) 33_656 6_556
Ge2 Ba2 Ge3 96.04(5) 29_556 6_556
Rh1 Ba2 Ge3 36.44(8) 33_656 6_556
Rh1 Ba2 Ge3 96.04(5) 29_556 6_556
Ge2 Ba2 Ge3 126.44(8) 9 6_556
Rh1 Ba2 Ge3 126.44(8) 9 6_556
Ge2 Ba2 Ge3 96.04(5) 5 6_556
Rh1 Ba2 Ge3 96.04(5) 5 6_556
Ge1 Ba2 Ge3 59.007(12) 37_666 6_556
Ge1 Ba2 Ge3 150.240(11) 27 6_556
Ge1 Ba2 Ge3 117.50(2) 39_656 6_556
Ge1 Ba2 Ge3 35.42(4) 26_556 6_556
Ge1 Ba2 Ge3 117.50(2) 14 6_556
Ge1 Ba2 Ge3 150.240(11) . 6_556
Ge1 Ba2 Ge3 59.007(12) 16_545 6_556
Ge1 Ba2 Ge3 35.42(4) 4_556 6_556
Ge4 Ba2 Ge3 91.88(4) 46_656 6_556
Ge4 Ba2 Ge3 4.15(7) 6_556 6_556
Ge4 Ba2 Ge3 91.88(4) 45_666 6_556
Ge4 Ba2 Ge3 158.7(2) 5 6_556
Ge3 Ba2 Ge3 91.27(2) 45_666 6_556
Ge3 Ba2 Ge3 162.88(15) 5 6_556
Ge3 Ba2 Ge3 91.27(2) 46_656 6_556
Ge4 Rh1 Ge4 109.42(6) 14 9
Ge4 Rh1 Ge4 109.58(12) 14 37_665
Ge4 Rh1 Ge4 109.42(6) 9 37_665
Ge4 Rh1 Ge4 109.42(6) 14 34_565
Ge4 Rh1 Ge4 109.58(12) 9 34_565
Ge4 Rh1 Ge4 109.42(6) 37_665 34_565
Ge4 Rh1 Ge3 0.10(9) 14 14
Ge4 Rh1 Ge3 109.37(2) 9 14
Ge4 Rh1 Ge3 109.68(5) 37_665 14
Ge4 Rh1 Ge3 109.37(2) 34_565 14
Ge4 Rh1 Ge3 109.37(2) 14 9
Ge4 Rh1 Ge3 0.10(9) 9 9
Ge4 Rh1 Ge3 109.37(2) 37_665 9
Ge4 Rh1 Ge3 109.68(5) 34_565 9
Ge3 Rh1 Ge3 109.31(3) 14 9
Ge4 Rh1 Ge3 109.37(2) 14 34_565
Ge4 Rh1 Ge3 109.68(5) 9 34_565
Ge4 Rh1 Ge3 109.37(2) 37_665 34_565
Ge4 Rh1 Ge3 0.10(9) 34_565 34_565
Ge3 Rh1 Ge3 109.31(3) 14 34_565
Ge3 Rh1 Ge3 109.79(7) 9 34_565
Ge4 Rh1 Ge3 109.68(5) 14 37_665
Ge4 Rh1 Ge3 109.37(2) 9 37_665
Ge4 Rh1 Ge3 0.10(9) 37_665 37_665
Ge4 Rh1 Ge3 109.37(2) 34_565 37_665
Ge3 Rh1 Ge3 109.79(7) 14 37_665
Ge3 Rh1 Ge3 109.31(3) 9 37_665
Ge3 Rh1 Ge3 109.31(3) 34_565 37_665
Ge4 Rh1 Ba2 170.21(6) 14 33_565
Ge4 Rh1 Ba2 65.94(4) 9 33_565
Ge4 Rh1 Ba2 80.21(6) 37_665 33_565
Ge4 Rh1 Ba2 65.94(4) 34_565 33_565
Ge3 Rh1 Ba2 170.11(3) 14 33_565
Ge3 Rh1 Ba2 66.01(2) 9 33_565
Ge3 Rh1 Ba2 66.01(2) 34_565 33_565
Ge3 Rh1 Ba2 80.11(3) 37_665 33_565
Ge4 Rh1 Ba2 65.94(4) 14 29_665
Ge4 Rh1 Ba2 170.21(6) 9 29_665
Ge4 Rh1 Ba2 65.94(4) 37_665 29_665
Ge4 Rh1 Ba2 80.21(6) 34_565 29_665
Ge3 Rh1 Ba2 66.01(2) 14 29_665
Ge3 Rh1 Ba2 170.11(3) 9 29_665
Ge3 Rh1 Ba2 80.11(3) 34_565 29_665
Ge3 Rh1 Ba2 66.01(2) 37_665 29_665
Ba2 Rh1 Ba2 120.0 33_565 29_665
Ge4 Rh1 Ba2 65.94(4) 14 5
Ge4 Rh1 Ba2 80.21(6) 9 5
Ge4 Rh1 Ba2 65.94(4) 37_665 5
Ge4 Rh1 Ba2 170.21(6) 34_565 5
Ge3 Rh1 Ba2 66.01(2) 14 5
Ge3 Rh1 Ba2 80.11(3) 9 5
Ge3 Rh1 Ba2 170.11(3) 34_565 5
Ge3 Rh1 Ba2 66.01(2) 37_665 5
Ba2 Rh1 Ba2 120.0 33_565 5
Ba2 Rh1 Ba2 90.0 29_665 5
Ge4 Rh1 Ba2 80.21(6) 14 9
Ge4 Rh1 Ba2 65.94(4) 9 9
Ge4 Rh1 Ba2 170.21(6) 37_665 9
Ge4 Rh1 Ba2 65.94(4) 34_565 9
Ge3 Rh1 Ba2 80.11(3) 14 9
Ge3 Rh1 Ba2 66.01(2) 9 9
Ge3 Rh1 Ba2 66.01(2) 34_565 9
Ge3 Rh1 Ba2 170.11(3) 37_665 9
Ba2 Rh1 Ba2 90.0 33_565 9
Ba2 Rh1 Ba2 120.0 29_665 9
Ba2 Rh1 Ba2 120.0 5 9
Ge4 Ge2 Ge4 109.42(6) 14 9
Ge4 Ge2 Ge4 109.58(12) 14 37_665
Ge4 Ge2 Ge4 109.42(6) 9 37_665
Ge4 Ge2 Ge4 109.42(6) 14 34_565
Ge4 Ge2 Ge4 109.58(12) 9 34_565
Ge4 Ge2 Ge4 109.42(6) 37_665 34_565
Ge4 Ge2 Ge3 0.10(9) 14 14
Ge4 Ge2 Ge3 109.37(2) 9 14
Ge4 Ge2 Ge3 109.68(5) 37_665 14
Ge4 Ge2 Ge3 109.37(2) 34_565 14
Ge4 Ge2 Ge3 109.37(2) 14 9
Ge4 Ge2 Ge3 0.10(9) 9 9
Ge4 Ge2 Ge3 109.37(2) 37_665 9
Ge4 Ge2 Ge3 109.68(5) 34_565 9
Ge3 Ge2 Ge3 109.31(3) 14 9
Ge4 Ge2 Ge3 109.37(2) 14 34_565
Ge4 Ge2 Ge3 109.68(5) 9 34_565
Ge4 Ge2 Ge3 109.37(2) 37_665 34_565
Ge4 Ge2 Ge3 0.10(9) 34_565 34_565
Ge3 Ge2 Ge3 109.31(3) 14 34_565
Ge3 Ge2 Ge3 109.79(7) 9 34_565
Ge4 Ge2 Ge3 109.68(5) 14 37_665
Ge4 Ge2 Ge3 109.37(2) 9 37_665
Ge4 Ge2 Ge3 0.10(9) 37_665 37_665
Ge4 Ge2 Ge3 109.37(2) 34_565 37_665
Ge3 Ge2 Ge3 109.79(7) 14 37_665
Ge3 Ge2 Ge3 109.31(3) 9 37_665
Ge3 Ge2 Ge3 109.31(3) 34_565 37_665
Ge4 Ge2 Ba2 170.21(6) 14 33_565
Ge4 Ge2 Ba2 65.94(4) 9 33_565
Ge4 Ge2 Ba2 80.21(6) 37_665 33_565
Ge4 Ge2 Ba2 65.94(4) 34_565 33_565
Ge3 Ge2 Ba2 170.11(3) 14 33_565
Ge3 Ge2 Ba2 66.01(2) 9 33_565
Ge3 Ge2 Ba2 66.01(2) 34_565 33_565
Ge3 Ge2 Ba2 80.11(3) 37_665 33_565
Ge4 Ge2 Ba2 65.94(4) 14 29_665
Ge4 Ge2 Ba2 170.21(6) 9 29_665
Ge4 Ge2 Ba2 65.94(4) 37_665 29_665
Ge4 Ge2 Ba2 80.21(6) 34_565 29_665
Ge3 Ge2 Ba2 66.01(2) 14 29_665
Ge3 Ge2 Ba2 170.11(3) 9 29_665
Ge3 Ge2 Ba2 80.11(3) 34_565 29_665
Ge3 Ge2 Ba2 66.01(2) 37_665 29_665
Ba2 Ge2 Ba2 120.0 33_565 29_665
Ge4 Ge2 Ba2 65.94(4) 14 5
Ge4 Ge2 Ba2 80.21(6) 9 5
Ge4 Ge2 Ba2 65.94(4) 37_665 5
Ge4 Ge2 Ba2 170.21(6) 34_565 5
Ge3 Ge2 Ba2 66.01(2) 14 5
Ge3 Ge2 Ba2 80.11(3) 9 5
Ge3 Ge2 Ba2 170.11(3) 34_565 5
Ge3 Ge2 Ba2 66.01(2) 37_665 5
Ba2 Ge2 Ba2 120.0 33_565 5
Ba2 Ge2 Ba2 90.0 29_665 5
Ge4 Ge2 Ba2 80.21(6) 14 9
Ge4 Ge2 Ba2 65.94(4) 9 9
Ge4 Ge2 Ba2 170.21(6) 37_665 9
Ge4 Ge2 Ba2 65.94(4) 34_565 9
Ge3 Ge2 Ba2 80.11(3) 14 9
Ge3 Ge2 Ba2 66.01(2) 9 9
Ge3 Ge2 Ba2 66.01(2) 34_565 9
Ge3 Ge2 Ba2 170.11(3) 37_665 9
Ba2 Ge2 Ba2 90.0 33_565 9
Ba2 Ge2 Ba2 120.0 29_665 9
Ba2 Ge2 Ba2 120.0 5 9
Ge1 Ge1 Ge3 108.55(13) 14 .
Ge1 Ge1 Ge3 108.55(13) 14 9
Ge3 Ge1 Ge3 110.38(13) . 9
Ge1 Ge1 Ge3 108.55(13) 14 5
Ge3 Ge1 Ge3 110.38(13) . 5
Ge3 Ge1 Ge3 110.38(13) 9 5
Ge1 Ge1 Ge4 101.8(2) 14 .
Ge3 Ge1 Ge4 6.92(9) . .
Ge3 Ge1 Ge4 112.18(14) 9 .
Ge3 Ge1 Ge4 114.85(16) 5 .
Ge1 Ge1 Ge4 101.8(2) 14 9
Ge3 Ge1 Ge4 114.85(16) . 9
Ge3 Ge1 Ge4 6.92(9) 9 9
Ge3 Ge1 Ge4 112.18(14) 5 9
Ge4 Ge1 Ge4 115.94(13) . 9
Ge1 Ge1 Ge4 101.8(2) 14 5
Ge3 Ge1 Ge4 112.18(14) . 5
Ge3 Ge1 Ge4 114.85(16) 9 5
Ge3 Ge1 Ge4 6.92(9) 5 5
Ge4 Ge1 Ge4 115.94(13) . 5
Ge4 Ge1 Ge4 115.94(13) 9 5
Ge1 Ge1 Ba1 180.00(5) 14 .
Ge3 Ge1 Ba1 71.45(13) . .
Ge3 Ge1 Ba1 71.45(13) 9 .
Ge3 Ge1 Ba1 71.45(13) 5 .
Ge4 Ge1 Ba1 78.2(2) . .
Ge4 Ge1 Ba1 78.2(2) 9 .
Ge4 Ge1 Ba1 78.2(2) 5 .
Ge1 Ge1 Ba2 71.983(10) 14 5
Ge3 Ge1 Ba2 172.09(5) . 5
Ge3 Ge1 Ba2 76.42(9) 9 5
Ge3 Ge1 Ba2 62.57(5) 5 5
Ge4 Ge1 Ba2 170.95(11) . 5
Ge4 Ge1 Ba2 72.32(12) 9 5
Ge4 Ge1 Ba2 60.37(7) 5 5
Ba1 Ge1 Ba2 108.017(10) . 5
Ge1 Ge1 Ba2 71.983(10) 14 .
Ge3 Ge1 Ba2 62.57(5) . .
Ge3 Ge1 Ba2 172.09(5) 9 .
Ge3 Ge1 Ba2 76.42(9) 5 .
Ge4 Ge1 Ba2 60.37(7) . .
Ge4 Ge1 Ba2 170.95(11) 9 .
Ge4 Ge1 Ba2 72.32(12) 5 .
Ba1 Ge1 Ba2 108.017(10) . .
Ba2 Ge1 Ba2 110.885(10) 5 .
Ge1 Ge1 Ba2 71.983(10) 14 9
Ge3 Ge1 Ba2 76.42(9) . 9
Ge3 Ge1 Ba2 62.57(5) 9 9
Ge3 Ge1 Ba2 172.09(5) 5 9
Ge4 Ge1 Ba2 72.32(12) . 9
Ge4 Ge1 Ba2 60.37(7) 9 9
Ge4 Ge1 Ba2 170.95(11) 5 9
Ba1 Ge1 Ba2 108.017(10) . 9
Ba2 Ge1 Ba2 110.885(10) 5 9
Ba2 Ge1 Ba2 110.885(10) . 9
Ge1 Ge1 Ba2 107.827(7) 14 33_565
Ge3 Ge1 Ba2 108.56(4) . 33_565
Ge3 Ge1 Ba2 2.55(3) 9 33_565
Ge3 Ge1 Ba2 112.87(9) 5 33_565
Ge4 Ge1 Ba2 110.15(6) . 33_565
Ge4 Ge1 Ba2 7.23(19) 9 33_565
Ge4 Ge1 Ba2 117.38(13) 5 33_565
Ba1 Ge1 Ba2 72.173(7) . 33_565
Ba2 Ge1 Ba2 78.367(1) 5 33_565
Ba2 Ge1 Ba2 169.6 . 33_565
Ba2 Ge1 Ba2 60.135(2) 9 33_565
Ge4 Ge3 Ge3 124.4(6) . 2
Ge4 Ge3 Ge1 106.0(4) . 28
Ge3 Ge3 Ge1 107.19(10) 2 28
Ge4 Ge3 Ge1 106.0(4) . .
Ge3 Ge3 Ge1 107.19(10) 2 .
Ge1 Ge3 Ge1 104.56(11) 28 .
Ge4 Ge3 Ge2 0.7(6) . 5
Ge3 Ge3 Ge2 125.11(3) 2 5
Ge1 Ge3 Ge2 105.56(14) 28 5
Ge1 Ge3 Ge2 105.56(14) . 5
Ge4 Ge3 Rh1 0.7(6) . 5
Ge3 Ge3 Rh1 125.11(3) 2 5
Ge1 Ge3 Rh1 105.56(14) 28 5
Ge1 Ge3 Rh1 105.56(14) . 5
Ge2 Ge3 Rh1 0.0 5 5
Ge4 Ge3 Ge4 118.6(7) . 2
Ge3 Ge3 Ge4 5.79(8) 2 2
Ge1 Ge3 Ge4 110.37(8) 28 2
Ge1 Ge3 Ge4 110.37(8) . 2
Ge2 Ge3 Ge4 119.32(10) 5 2
Rh1 Ge3 Ge4 119.32(10) 5 2
Ge4 Ge3 Ba1 166.1(6) . .
Ge3 Ge3 Ba1 69.52(3) 2 .
Ge1 Ge3 Ba1 66.52(12) 28 .
Ge1 Ge3 Ba1 66.52(12) . .
Ge2 Ge3 Ba1 165.37(6) 5 .
Rh1 Ge3 Ba1 165.37(6) 5 .
Ge4 Ge3 Ba1 75.31(7) 2 .
Ge4 Ge3 Ba2 73.8(4) . .
Ge3 Ge3 Ba2 69.96(7) 2 .
Ge1 Ge3 Ba2 175.68(5) 28 .
Ge1 Ge3 Ba2 79.547(19) . .
Ge2 Ge3 Ba2 74.27(10) 5 .
Rh1 Ge3 Ba2 74.27(10) 5 .
Ge4 Ge3 Ba2 66.51(10) 2 .
Ba1 Ge3 Ba2 114.60(11) . .
Ge4 Ge3 Ba2 73.8(4) . 25_556
Ge3 Ge3 Ba2 69.96(7) 2 25_556
Ge1 Ge3 Ba2 79.547(19) 28 25_556
Ge1 Ge3 Ba2 175.68(5) . 25_556
Ge2 Ge3 Ba2 74.27(10) 5 25_556
Rh1 Ge3 Ba2 74.27(10) 5 25_556
Ge4 Ge3 Ba2 66.51(10) 2 25_556
Ba1 Ge3 Ba2 114.60(11) . 25_556
Ba2 Ge3 Ba2 96.32(7) . 25_556
Ge4 Ge3 Ba2 64.2(6) . 9
Ge3 Ge3 Ba2 171.44(8) 2 9
Ge1 Ge3 Ba2 68.16(5) 28 9
Ge1 Ge3 Ba2 68.16(5) . 9
Ge2 Ge3 Ba2 63.45(8) 5 9
Rh1 Ge3 Ba2 63.45(8) 5 9
Ge4 Ge3 Ba2 177.23(9) 2 9
Ba1 Ge3 Ba2 101.92(6) . 9
Ba2 Ge3 Ba2 115.09(10) . 9
Ba2 Ge3 Ba2 115.09(10) 25_556 9
Ge3 Ge4 Ge2 179.2(7) . 5
Ge3 Ge4 Rh1 179.2(7) . 5
Ge2 Ge4 Rh1 0.0 5 5
Ge3 Ge4 Ge1 67.1(4) . 28
Ge2 Ge4 Ge1 112.4(2) 5 28
Rh1 Ge4 Ge1 112.4(2) 5 28
Ge3 Ge4 Ge1 67.1(4) . .
Ge2 Ge4 Ge1 112.4(2) 5 .
Rh1 Ge4 Ge1 112.4(2) 5 .
Ge1 Ge4 Ge1 98.6(2) 28 .
Ge3 Ge4 Ge3 49.8(6) . 2
Ge2 Ge4 Ge3 131.00(12) 5 2
Rh1 Ge4 Ge3 131.00(12) 5 2
Ge1 Ge4 Ge3 98.58(19) 28 2
Ge1 Ge4 Ge3 98.58(19) . 2
Ge3 Ge4 Ge4 55.6(6) . 2
Ge2 Ge4 Ge4 125.21(6) 5 2
Rh1 Ge4 Ge4 125.21(6) 5 2
Ge1 Ge4 Ge4 102.27(15) 28 2
Ge1 Ge4 Ge4 102.27(15) . 2
Ge3 Ge4 Ge4 5.79(8) 2 2
Ge3 Ge4 Ba2 101.1(4) . .
Ge2 Ge4 Ba2 79.43(16) 5 .
Rh1 Ge4 Ba2 79.43(16) 5 .
Ge1 Ge4 Ba2 167.5(3) 28 .
Ge1 Ge4 Ba2 79.752(19) . .
Ge3 Ge4 Ba2 69.57(11) 2 .
Ge4 Ge4 Ba2 66.27(12) 2 .
Ge3 Ge4 Ba2 101.1(4) . 25_556
Ge2 Ge4 Ba2 79.43(16) 5 25_556
Rh1 Ge4 Ba2 79.43(16) 5 25_556
Ge1 Ge4 Ba2 79.752(19) 28 25_556
Ge1 Ge4 Ba2 167.5(3) . 25_556
Ge3 Ge4 Ba2 69.57(10) 2 25_556
Ge4 Ge4 Ba2 66.27(12) 2 25_556
Ba2 Ge4 Ba2 99.15(9) . 25_556
Ge3 Ge4 Ba1 12.8(6) . .
Ge2 Ge4 Ba1 166.43(10) 5 .
Rh1 Ge4 Ba1 166.43(10) 5 .
Ge1 Ge4 Ba1 60.34(18) 28 .
Ge1 Ge4 Ba1 60.34(18) . .
Ge3 Ge4 Ba1 62.57(10) 2 .
Ge4 Ge4 Ba1 68.36(5) 2 .
Ba2 Ge4 Ba1 108.92(18) . .
Ba2 Ge4 Ba1 108.92(18) 25_556 .
Ge3 Ge4 Ba2 111.7(6) . 9
Ge2 Ge4 Ba2 67.50(14) 5 9
Rh1 Ge4 Ba2 67.50(14) 5 9
Ge1 Ge4 Ba2 69.94(6) 28 9
Ge1 Ge4 Ba2 69.94(6) . 9
Ge3 Ge4 Ba2 161.5(2) 2 9
Ge4 Ge4 Ba2 167.29(13) 2 9
Ba2 Ge4 Ba2 120.29(15) . 9
Ba2 Ge4 Ba2 120.29(15) 25_556 9
Ba1 Ge4 Ba2 98.93(11) . 9
Ge3 Ge4 Ba2 173.0(6) . 33_566
Ge2 Ge4 Ba2 6.21(4) 5 33_566
Rh1 Ge4 Ba2 6.21(4) 5 33_566
Ge1 Ge4 Ba2 108.8(2) 28 33_566
Ge1 Ge4 Ba2 108.8(2) . 33_566
Ge3 Ge4 Ba2 137.20(10) 2 33_566
Ge4 Ge4 Ba2 131.42(3) 2 33_566
Ba2 Ge4 Ba2 83.39(16) . 33_566
Ba2 Ge4 Ba2 83.39(16) 25_556 33_566
Ba1 Ge4 Ba2 160.23(6) . 33_566
Ba2 Ge4 Ba2 61.30(12) 9 33_566
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 Ge1 3.4004(10) .
Ba1 Ge1 3.4004(10) 25
Ba1 Ge1 3.4004(10) 28
Ba1 Ge1 3.4004(10) 4
Ba1 Ge1 3.4004(10) 27
Ba1 Ge1 3.4004(10) 3
Ba1 Ge1 3.4004(10) 26
Ba1 Ge1 3.4004(10) 2
Ba1 Ge3 3.515(6) .
Ba1 Ge3 3.515(6) 33
Ba1 Ge3 3.515(6) 29
Ba1 Ge3 3.515(6) 25
Ba2 Ge4 3.512(2) 41_666
Ba2 Ge4 3.512(2) 2
Ba2 Ge4 3.512(2) .
Ba2 Ge4 3.512(2) 42_666
Ba2 Ge4 3.512(2) 18_545
Ba2 Ge4 3.512(2) 26_556
Ba2 Ge4 3.512(2) 25_556
Ba2 Ge4 3.512(2) 17_545
Ba2 Ge3 3.588(2) 41_666
Ba2 Ge3 3.588(2) 2
Ba2 Ge3 3.588(2) 42_666
Ba2 Ge3 3.588(2) .
Ba2 Ge3 3.588(2) 25_556
Ba2 Ge3 3.588(2) 17_545
Ba2 Ge3 3.588(2) 26_556
Ba2 Ge3 3.588(2) 18_545
Ba2 Ge2 3.7804(7) 33_656
Ba2 Ge2 3.7804(7) 29_556
Ba2 Rh1 3.7804(7) 33_656
Ba2 Rh1 3.7804(7) 29_556
Ba2 Ge2 3.7804(7) 9
Ba2 Rh1 3.7804(7) 9
Ba2 Ge2 3.7804(7) 5
Ba2 Rh1 3.7804(7) 5
Ba2 Ge1 3.9753(8) 37_666
Ba2 Ge1 3.9753(8) 27
Ba2 Ge1 3.9753(8) 39_656
Ba2 Ge1 3.9753(8) 26_556
Ba2 Ge1 3.9753(8) 14
Ba2 Ge1 3.9753(8) .
Ba2 Ge1 3.9753(8) 16_545
Ba2 Ge1 3.9753(8) 4_556
Ba2 Ge4 4.032(4) 46_656
Ba2 Ge4 4.032(4) 6_556
Ba2 Ge4 4.032(4) 45_666
Ba2 Ge4 4.032(4) 5
Ba2 Ge3 4.163(3) 45_666
Ba2 Ge3 4.163(3) 5
Ba2 Ge3 4.163(3) 46_656
Ba2 Ge3 4.163(3) 6_556
Rh1 Ge4 2.186(10) 14
Rh1 Ge4 2.186(10) 9
Rh1 Ge4 2.186(10) 37_665
Rh1 Ge4 2.186(10) 34_565
Rh1 Ge3 2.510(6) 14
Rh1 Ge3 2.510(6) 9
Rh1 Ge3 2.510(6) 34_565
Rh1 Ge3 2.510(6) 37_665
Rh1 Ba2 3.7804(7) 33_565
Rh1 Ba2 3.7804(7) 29_665
Rh1 Ba2 3.7804(7) 5
Rh1 Ba2 3.7804(7) 9
Ge2 Ge4 2.186(10) 14
Ge2 Ge4 2.186(10) 9
Ge2 Ge4 2.186(10) 37_665
Ge2 Ge4 2.186(10) 34_565
Ge2 Ge3 2.510(6) 14
Ge2 Ge3 2.510(6) 9
Ge2 Ge3 2.510(6) 34_565
Ge2 Ge3 2.510(6) 37_665
Ge2 Ba2 3.7804(7) 33_565
Ge2 Ba2 3.7804(7) 29_665
Ge2 Ba2 3.7804(7) 5
Ge2 Ba2 3.7804(7) 9
Ge1 Ge1 2.4592(15) 14
Ge1 Ge3 2.4820(19) .
Ge1 Ge3 2.4820(19) 9
Ge1 Ge3 2.4820(19) 5
Ge1 Ge4 2.590(4) .
Ge1 Ge4 2.590(4) 9
Ge1 Ge4 2.590(4) 5
Ge1 Ba2 3.9753(8) 5
Ge1 Ba2 3.9753(8) 9
Ge1 Ba2 6.0659(12) 33_565
Ge3 Ge4 0.325(5) .
Ge3 Ge3 2.459(7) 2
Ge3 Ge1 2.4820(19) 28
Ge3 Ge2 2.510(6) 5
Ge3 Rh1 2.510(6) 5
Ge3 Ge4 2.656(9) 2
Ge3 Ba2 3.588(2) 25_556
Ge3 Ba2 4.163(3) 9
Ge4 Ge2 2.186(10) 5
Ge4 Rh1 2.186(10) 5
Ge4 Ge1 2.590(4) 28
Ge4 Ge3 2.656(9) 2
Ge4 Ge4 2.826(12) 2
Ge4 Ba2 3.512(2) 25_556
Ge4 Ba2 4.032(4) 9
Ge4 Ba2 5.946(10) 33_566
